Solution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.


 Matilda Crawford
 1 years ago
 Views:
Transcription
1 14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius r). Now differentiate this expression with respect to a (per Equation 10.2) and solve for both the critical cube edge length, a*, and also ΔG*. (b) Is ΔG* greater for a cube or a sphere? Why? (a) This problem first asks that we rewrite the expression for the total free energy change for nucleation (analogous to Equation 10.1) for the case of a cubic nucleus of edge length a. The volume of such a cubic radius is a 3, whereas the total surface area is 6a 2 (since there are six faces each of which has an area of a 2 ). Thus, the expression for ΔG is as follows: ΔG = a 3 ΔG v + 6a 2 γ Differentiation of this expression with respect to a is as d ΔG da = d(a3 ΔG v ) + d(6a2 γ) da da = 3a 2 ΔG v + 12a γ If we set this expression equal to zero as 3a 2 ΔG v + 12a γ=0 and then solve for a (= a*), we have a *= 4 γ ΔG v Substitution of this expression for a in the above expression for ΔG yields an equation for ΔG* as ΔG *=(a*) 3 ΔG v + 6(a*) 2 γ
2 = 4 γ 3 ΔG ΔG v + 6 γ v 4 γ 2 ΔG v = 32 γ3 (ΔG v ) 2 γ (b) ΔG v for a cube i.e., 3 (32) (ΔG v ) 2 16 π γ is greater that for a sphere i.e., 3 3 (ΔG v ) 2 γ 3 (16.8) (ΔG v ) 2. The reason for this is that surfacetovolume ratio of a cube is greater than for a sphere. = Question 10.3: If copper (which has a melting point of 1085 C) homogeneously nucleates at 849 C, calculate the critical radius given values of J/m 3 and J/m 2, respectively, for the latent heat of fusion and the surface free energy. This problem states that copper homogeneously nucleates at 849 C, and that we are to calculate the critical radius given the latent heat of fusion ( J/m 3 ) and the surface free energy (0.200 J/m 2 ). Solution to this problem requires the utilization of Equation 10.6 as r * = 2 γt m 1 ΔH f T m T = (2)(0.200 J / m2 )( K) J/m C 849 C = m = 1.30 nm
3 Question 10.4: (a) For the solidification of iron, calculate the critical radius r* and the activation free energy ΔG* if nucleation is homogeneous. Values for the latent heat of fusion and surface free energy are J/m 3 and J/m 2, respectively. Use the supercooling value found in Table (b) Now calculate the number of atoms found in a nucleus of critical size. Assume a lattice parameter of nm for solid iron at its melting temperature. (a) This portion of the problem asks that we compute r* and ΔG* for the homogeneous nucleation of the solidification of Fe. First of all, Equation 10.6 is used to compute the critical radius. The melting temperature for iron, found inside the front cover is 1538 C; also values of ΔH f ( J/m 3 ) and γ (0.204 J/m 2 ) are given in the problem statement, and the supercooling value found in Table 10.1 is 295 C (or 295 K). Thus, from Equation 10.6 we have r * = 2γT m 1 ΔH f T m T = (2)(0.204 J / m2 )( K) J/m K = m = 1.35 nm For computation of the activation free energy, Equation 10.7 is employed. Thus ΔG * = 16 πγ3 T 2 m 1 3ΔH 2 f (T m T) 2 = (16)(π)(0.204 J /m2 ) 3 ( K) 2 1 (3)( J/m 3 ) 2 (295 K) 2 = J (b) In order to compute the number of atoms in a nucleus of critical size (assuming a spherical nucleus of radius r*), it is first necessary to determine the number of unit cells, which we then multiply by the number of atoms per unit cell. The number of unit cells found in this critical nucleus is just the ratio of critical nucleus and unit cell
4 volumes. Inasmuch as iron has the BCC crystal structure, its unit cell volume is just a 3 where a is the unit cell length (i.e., the lattice parameter); this value is nm, as cited in the problem statement. Therefore, the number of unit cells found in a radius of critical size is just # unit cells /particle = 4 πr *3 3 a 3 = 4 (π)(1.35 nm) 3 3 (0.292 nm) 3 = 414 unit cells Inasmuch as 2 atoms are associated with each BCC unit cell, the total number of atoms per critical nucleus is just (414 unit cells /critical nucleus)(2 atoms /unit cell) = 828 atoms /critical nucleus
5 Question 10.5: (a) Assume for the solidification of iron (Problem 10.4) that nucleation is homogeneous, and the number of stable nuclei is 10 6 nuclei per cubic meter. Calculate the critical radius and the number of stable nuclei that exist at the following degrees of supercooling: 200 K and 300 K. (b) What is significant about the magnitudes of these critical radii and the numbers of stable nuclei? (a) For this part of the problem we are asked to calculate the critical radius for the solidification of iron (per Problem 10.4), for 200 K and 300 K degrees of supercooling, and assuming that the there are 10 6 nuclei per meter cubed for homogeneous nucleation. In order to calculate the critical radii, we replace the T m T term in Equation 10.6 by the degree of supercooling (denoted as ΔT) cited in the problem. For 200 K supercooling, r* 2 γt 200 = m 1 ΔH f ΔT = (2)(0.204 J / m2 )( K) J/m K = m = 2.00 nm And, for 300 K supercooling, r* (2)(0.204 J / m 2 )( K) = J/m K = m = 1.33 nm In order to compute the number of stable nuclei that exist at 200 K and 300 K degrees of supercooling, it is necessary to use Equation However, we must first determine the value of K 1 in Equation 10.8, which in turn requires that we calculate ΔG* at the homogeneous nucleation temperature using Equation 10.7; this was done in Problem 10.4, and yielded a value of ΔG* = J. Now for the computation of K 1, using the value of n* for at the homogenous nucleation temperature (10 6 nuclei/m 3 ): K 1 = n * exp ΔG * kt
6 = exp 10 6 nuclei / m J ( J / atom K)(1538 C 295 C) = nuclei/m 3 Now for 200 K supercooling, it is first necessary to recalculate the value ΔG* of using Equation 10.7, where, again, the T m T term is replaced by the number of degrees of supercooling, denoted as ΔT, which in this case is 200 K. Thus ΔG* 200 = 16 πγ3 T 2 m 1 3ΔH 2 f (ΔT) 2 = (16)(π)(0.204 J / m2 ) 3 ( K) 2 1 (3)( J/m 3 ) 2 (200 K) 2 = J And, from Equation 10.8, the value of n* is n* 200 = K 1 exp ΔG * 200 kt = ( nuclei / m )exp 18 J ( J /atom K) (1538 K 200 K) = stable nuclei Now, for 300 K supercooling the value of ΔG* is equal to ΔG* (16)(π)(0.204 J /m = ) 3 ( K) 2 1 (3)( J/m 3 ) 2 (300 K) 2 = J
7 from which we compute the number of stable nuclei at 300 K of supercooling as * = K 1 exp ΔG * 300 kt n 300 n* = ( nuclei / m )exp 18 J ( J / atom K) (1538 K 300 K) = stable nuclei (b) Relative to critical radius, r* for 300 K supercooling is slightly smaller that for 200 K (1.33 nm versus 2.00 nm). [From Problem 10.4, the value of r* at the homogeneous nucleation temperature (295 K) was 1.35 nm.] More significant, however, are the values of n* at these two degrees of supercooling, which are dramatically different stable nuclei at ΔT = 200 K, versus stable nuclei at ΔT = 300 K!
8 Question 10.6: For some transformation having kinetics that obey the Avrami equation (Equation 10.17), the parameter n is known to have a value of 1.7. If, after 100 s, the reaction is 50% complete, how long (total time) will it take the transformation to go to 99% completion? This problem calls for us to compute the length of time required for a reaction to go to 99% completion. It first becomes necessary to solve for the parameter k in Equation In order to do this it is best manipulate the equation such that k is the dependent variable. We first rearrange Equation as exp( kt n ) = 1 y and then take natural logarithms of both sides: kt n = ln (1 y) Now solving for k gives k = ln (1 y) t n And, from the problem statement, for y = 0.50 when t = 100 s and given that n = 1.7, the value of k is equal to k = ln (1 0.5) (100 s) 1.7 = We now want to manipulate Equation such that t is the dependent variable. The above equation may be written in the form: t n = ln (1 y) k And solving this expression for t leads to t = ln (1 y) k 1/n
9 Now, using this equation and the value of k determined above, the time to 99% transformation completion is equal to t = ln (1 0.99) /1.7 = 305 s
10 Question 10.8: It is known that the kinetics of recrystallization for some alloy obey the Avrami equation and that the value of n in the exponential is 2.5. If, at some temperature, the fraction recrystallized is 0.40 after 200 min, determine the rate of recrystallization at this temperature. This problem gives us the value of y (0.40) at some time t (200 min), and also the value of n (2.5) for the recrystallization of an alloy at some temperature, and then asks that we determine the rate of recrystallization at this same temperature. It is first necessary to calculate the value of k. We first rearrange Equation as exp( kt n ) = 1 y and then take natural logarithms of both sides: kt n = ln (1 y) Now solving for k gives k = ln (1 y) t n which, using the values cited above for y, n, and t yields ln (1 0.40) k = = (200 min) 2.5 At this point we want to compute t 0.5, the value of t for y = 0.5, which means that it is necessary to establish a form of Equation in which t is the dependent variable. From one of the above equations t n = ln (1 y) k And solving this expression for t leads to
11 1/n ln (1 y) t = k For t 0.5, this equation takes the form t 0.5 = ln (1 0.5) k 1/n and incorporation of the value of k determined above, as well as the value of n cited in the problem statement (2.5), then t 0.5 is equal to t 0.5 = ln (1 0.5) /2.5 = min Therefore, from Equation 10.18, the rate is just rate = 1 t 0.5 = min = (min) 1
12 Question 10.9: The kinetics of the austenitetopearlite transformation obey the Avrami relationship. Using the fraction transformed time data given here, determine the total time required for 95% of the austenite to transform to pearlite: Fraction Transformed Time (s) The first thing necessary is to set up two expressions of the form of Equation 10.17, and then to solve simultaneously for the values of n and k. In order to expedite this process, we will rearrange and do some algebraic manipulation of Equation First of all, we rearrange as follows: 1 y = exp ( kt n ) Now taking natural logarithms ln (1 y) = kt n Or ln (1 y) = kt n which may also be expressed as 1 ln = kt n 1 y Now taking natural logarithms again, leads to 1 ln ln = ln k + n ln t 1 y
13 which is the form of the equation that we will now use. Using values cited in the problem statement, the two equations are thus 1 ln ln = ln k + n ln (12.6 s) ln ln = ln k + n ln (28.2 s) Solving these two expressions simultaneously for n and k yields n = and k = Now it becomes necessary to solve for the value of t at which y = One of the above equations viz ln (1 y) = kt n may be rewritten as t n = ln (1 y) k And solving for t leads to t = ln (1 y) k 1/n Now incorporating into this expression values for n and k determined above, the time required for 95% austenite transformation is equal to 1/2.453 ln (1 0.95) t = = 35.7 s
14 Question 10.11: (a) From the curves shown in Figure and using Equation 10.18, determine the rate of recrystallization for pure copper at the several temperatures. (b) Make a plot of ln(rate) versus the reciprocal of temperature (in K 1 ), and determine the activation energy for this recrystallization process. (See Section 5.5.) (c) By extrapolation, estimate the length of time required for 50% recrystallization at room temperature, 20 C (293 K). This problem asks us to consider the percent recrystallized versus logarithm of time curves for copper shown in Figure (a) The rates at the different temperatures are determined using Equation 10.18, which rates are tabulated below: Temperature ( C) Rate (min) (b) These data are plotted below.
15 The activation energy, Q, is related to the slope of the line drawn through the data points as Q = Slope (R) where R is the gas constant. The slope of this line is equal to Slope = Δ ln rate Δ 1 T = ln rate 1 ln rate 2 1 T 1 1 T 2 Let us take 1/T 1 = K 1 and 1/T 2 = K 1 ; the corresponding ln rate values are ln rate 1 = 2.6 and ln rate 2 = Thus, using these values, the slope is equal to Slope = 2.6 ( 9.4) K K 1 = K And, finally the activation energy is Q = (Slope)(R) = ( K 1 )(8.31 J/mol K) = 94,150 J/mol
16 (c) At room temperature (20 C), 1/T = 1/( K) = K 1. Extrapolation of the data in the plot to this 1/T value gives ln (rate) 12.8 which leads to rate exp ( 12.8) = (min) 1 But since rate = 1 t 0.5 t 0.5 = 1 rate = (min) 1 = min = 250 days
17 Question 10.14: (a) Briefly describe the phenomena of superheating and supercooling. (b) Why do these phenomena occur? (a) Superheating and supercooling correspond, respectively, to heating or cooling above or below a phase transition temperature without the occurrence of the transformation. (b) These phenomena occur because right at the phase transition temperature, the driving force is not sufficient to cause the transformation to occur. The driving force is enhanced during superheating or supercooling. Question 10.15: Suppose that a steel of eutectoid composition is cooled to 550 C (1020 F) from 760 C (1400 F) in less than 0.5 s and held at this temperature. (a) How long will it take for the austenitetopearlite reaction to go to 50% completion? To 100% completion? (b) Estimate the hardness of the alloy that has completely transformed to pearlite. We are called upon to consider the isothermal transformation of an ironcarbon alloy of eutectoid composition. (a) From Figure 10.22, a horizontal line at 550 C intersects the 50% and reaction completion curves at about 2.5 and 6 seconds, respectively; these are the times asked for in the problem statement. (b) The pearlite formed will be fine pearlite. From Figure 10.30a, the hardness of an alloy of composition 0.76 wt% C that consists of fine pearlite is about 265 HB (27 HRC). Question 10.16: Briefly cite the differences between pearlite, bainite, and spheroidite relative to microstructure and mechanical properties. The microstructures of pearlite, bainite, and spheroidite all consist of αferrite and cementite phases. For pearlite, the two phases exist as layers which alternate with one another. Bainite consists of very fine and parallel needleshaped particles of cementite that are surrounded an αferrite matrix. For spheroidite, the matrix is ferrite, and the cementite phase is in the shape of sphereshaped particles. Bainite is harder and stronger than pearlite, which, in turn, is harder and stronger than spheroidite.
18 Question 10.17: What is the driving force for the formation of spheroidite? The driving force for the formation of spheroidite is the net reduction in ferritecementite phase boundary area. Question 10.18: Using the isothermal transformation diagram for an iron carbon alloy of eutectoid composition (Figure 10.22), specify the nature of the final microstructure (in terms of microconstituents present and approximate percentages of each) of a small specimen that has been subjected to the following time temperature treatments. In each case assume that the specimen begins at 760 C (1400 F) and that it has been held at this temperature long enough to have achieved a complete and homogeneous austenitic structure. (a) Cool rapidly to 700 C (1290 F), hold for 10 4 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
19 After cooling and holding at 700 C for 10 4 s, approximately 50% of the specimen has transformed to coarse pearlite. Upon cooling to room temperature, the remaining 50% transforms to martensite. Hence, the final microstructure consists of about 50% coarse pearlite and 50% martensite. (b) Reheat the specimen in part (a) to 700 C (1290 F) for 20 h. spheroidite. Heating to 700 C for 20 h the specimen in part (a) will transform the coarse pearlite and martensite to (c) Rapidly cool to 600 C (1110 F), hold for 4 s, rapidly cool to 450 C (840 F), hold for 10 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
20 After cooling to and holding at 600 C for 4 s, approximately 50% of the specimen has transformed to pearlite (medium). During the rapid cooling to 450 C no transformations occur. At 450 C we start timing again at zero time; while holding at 450 C for 10 s, approximately 50 percent of the remaining unreacted 50% (or 25% of the original specimen) will transform to bainite. And upon cooling to room temperature, the remaining 25% of the original specimen transforms to martensite. Hence, the final microstructure consists of about 50% pearlite (medium), 25% bainite, and 25% martensite. (d) Cool rapidly to 400 C (750 F), hold for 2 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment. After cooling to and holding at 400 C for 2 s, no of the transformation begin lines have been crossed, and therefore, the specimen is 100% austenite. Upon cooling rapidly to room temperature, all of the specimen transforms to martensite, such that the final microstructure is 100% martensite.
21 (e) Cool rapidly to 400 C (750 F), hold for 20 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment. After cooling and holding at 400 C for 20 s, approximately 40% of the specimen has transformed to bainite. Upon cooling to room temperature, the remaining 60% transforms to martensite. Hence, the final microstructure consists of about 40% bainite and 60% martensite. (f) Cool rapidly to 400 C (750 F), hold for 200 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
22 After cooling and holding at 400 C for 200 s, the entire specimen has transformed to bainite. Therefore, during the cooling to room temperature no additional transformations will occur. Hence, the final microstructure consists of 100% bainite. (g) Rapidly cool to 575 C (1065 F), hold for 20 s, rapidly cool to 350 C (660 F), hold for 100 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
23 After cooling and holding at 575 C for 20 s, the entire specimen has transformed to fine pearlite. Therefore, during the second heat treatment at 350 C no additional transformations will occur. Hence, the final microstructure consists of 100% fine pearlite. (h) Rapidly cool to 250 C (480 F), hold for 100 s, then quench to room temperature in water. Reheat to 315 C (600 F) for 1 h and slowly cool to room temperature. Below is Figure upon which is superimposed the above heat treatment.
24 After cooling and holding at 250 C for 100 s, no transformations will have occurred at this point, the entire specimen is still austenite. Upon rapidly cooling to room temperature in water, the specimen will completely transform to martensite. The second heat treatment (at 315 C for 1 h) not shown on the above plot will transform the material to tempered martensite. Hence, the final microstructure is 100% tempered martensite.
25 Question 10.20: Using the isothermal transformation diagram for a 0.45 wt% C steel alloy (Figure 10.39), determine the final microstructure (in terms of just the microconstituents present) of a small specimen that has been subjected to the following timetemperature treatments. In each case assume that the specimen begins at 845 C (1550 F), and that it has been held at this temperature long enough to have achieved a complete and homogeneous austenitic structure. (a) Rapidly cool to 250 C (480 F), hold for 10 3 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment. While rapidly cooling to 250 C about 80% of the specimen transforms to martensite; during the 1000 s isothermal treatment at 250 C no additional transformations occur. During the final cooling to room temperature, the untransformed austenite also transforms to martensite. Hence, the final microstructure consists of 100% martensite. (b) Rapidly cool to 700 C (1290 F), hold for 30 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
26 After cooling to and holding at 700 C for 30 s, a portion of specimen has transformed to proeutectoid ferrite. While cooling to room temperature, the remainder of the specimen transforms to martensite. Hence, the final microstructure consists proeutectoid ferrite and martensite. (c) Rapidly cool to 400 C (750 F), hold for 500 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
27 After cooling to and holding at 400 C for 500 s, all of the specimen has transformed to bainite. Hence, the final microstructure consists of 100% bainite. (d) Rapidly cool to 700 C (1290 F), hold at this temperature for 10 5 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
28 After cooling to and while holding at 700 C the specimen first transforms to proeutectoid ferrite and coarse pearlite. Continued heat treating at 700 C for 10 5 s results in a further transformation into spheroidite. Hence, the final microstructure consists of 100% spheroidite. (e) Rapidly cool to 650 C (1200 F), hold at this temperature for 3 s, rapidly cool to 400 C (750 F), hold for 10 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
29 After cooling to and holding at 650 C for 3 s, some of the specimen first transformers to proeutectoid ferrite and then to pearlite (medium). During the second stage of the heat treatment at 400 C, some (but not all) of the remaining unreacted austenite transforms to bainite. As a result of the final quenching, all of the remaining austenite transforms to martensite. Hence, the final microstructure consists of ferrite, pearlite (medium), bainite, and martensite. (f) Rapidly cool to 450 C (840 F), hold for 10 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
30 After cooling to and holding at 450 C for 10 s, a portion of the specimen first transformers to bainite. During the quenching to room temperature, the remainder of the specimen transforms to martensite. Hence, the final microstructure consists of bainite and martensite. (g) Rapidly cool to 625 C (1155 F), hold for 1 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
31 After cooling to and holding at 625 C for 1 s, a portion of the specimen first transformers to proeutectoid ferrite and pearlite. During the quenching to room temperature, the remainder of the specimen transforms to martensite. Hence, the final microstructure consists of ferrite, pearlite, and martensite. (h) Rapidly cool to 625 C (1155 F), hold at this temperature for 10 s, rapidly cool to 400 C (750 F), hold at this temperature for 5 s, then quench to room temperature. Below is Figure upon which is superimposed the above heat treatment.
32 After cooling to and holding at 625 C for 10 s, all of the specimen transformers to proeutectoid ferrite and pearlite. During the second part of the heat treatment at 400 C no additional transformation will occur. Hence, the final microstructure consists of ferrite and pearlite.
33 Question 10.23: Name the microstructural products of eutectoid iron carbon alloy (0.76 wt% C) specimens that are first completely transformed to austenite, then cooled to room temperature at the following rates: (a) 200 C/s, (b) 100 C/s, and (c) 20 C/s. We are called upon to name the microstructural products that form for specimens of an ironcarbon alloy of eutectoid composition that are continuously cooled to room temperature at a variety of rates. Figure is used in these determinations. (a) At a rate of 200 C/s, only martensite forms. (b) At a rate of 100 C/s, both martensite and pearlite form. (c) At a rate of 20 C/s, only fine pearlite forms. Question 10.24: Figure shows the continuous cooling transformation diagram for a 1.13 wt% C ironcarbon alloy. Make a copy of this figure and then sketch and label continuous cooling curves to yield the following microstructures: (a) Fine pearlite and proeutectoid cementite (b) Martensite (c) Martensite and proeutectoid cementite (d) Coarse pearlite and proeutectoid cementite (e) Martensite, fine pearlite, and proeutectoid cementite Below is shown a continuous cooling transformation diagram for a 1.13 wt% C ironcarbon alloy, with continuous cooling paths that will produce (a) fine pearlite and proeutectoid cementite; (b) martensite; (c) martensite and proeutectoid cementite; (d) coarse pearlite and proeutectoid cementite; and (e) martensite, fine pearlite, and proeutectoid cementite.
34 Question 10.28: Briefly describe the simplest continuous cooling heat treatment procedure that would be used in converting a 4340 steel from one microstructure to another. (a) (Martensite + bainite) to (ferrite + pearlite) (b) (Martensite + bainite) to spheroidite (c) (Martensite + bainite) to (martensite + bainite + ferrite) This problem asks that we briefly describe the simplest continuous cooling heat treatment procedure that would be used in converting a 4340 steel from one microstructure to another. Solutions to this problem require the use of Figure (a) In order to convert from (martensite + bainite) to (ferrite + pearlite) it is necessary to heat above about 720 C, allow complete austenitization, then cool to room temperature at a rate slower than C/s. (b) To convert from (martensite + bainite) to spheroidite the alloy must be heated to about 700 C for several hours. (c) In order to convert from (martensite + bainite) to (martensite + bainite + ferrite) it is necessary to heat to above about 720 C, allow complete austenitization, then cool to room temperature at a rate between 0.3 C/s and 0.02 C/s.
35 Question 10.32: Rank the following iron carbon alloys and associated microstructures from the highest to the lowest tensile strength: (a) 0.25 wt%c with spheroidite, (b) 0.25 wt%c with coarse pearlite, (c) 0.60 wt%c with fine pearlite, and (d) 0.60 wt%c with coarse pearlite. Justify this ranking. This problem asks us to rank four ironcarbon alloys of specified composition and microstructure according to hardness. This ranking is as follows: 0.60 wt% C, fine pearlite 0.60 wt% C, coarse pearlite 0.25 wt% C, coarse pearlite 0.25 wt% C, spheroidite The 0.25 wt% C, coarse pearlite is stronger than the 0.25 wt% C, spheroidite since coarse pearlite is stronger than spheroidite; the composition of the alloys is the same. The 0.60 wt% C, coarse pearlite is stronger than the 0.25 wt% C, coarse pearlite, since increasing the carbon content increases the strength. Finally, the 0.60 wt% C, fine pearlite is stronger than the 0.60 wt% C, coarse pearlite inasmuch as the strength of fine pearlite is greater than coarse pearlite because of the many more ferritecementite phase boundaries in fine pearlite. Question 10.33: Briefly explain why the hardness of tempered martensite diminishes with tempering time (at constant temperature) and with increasing temperature (at constant tempering time). This question asks for an explanation as to why the hardness of tempered martensite diminishes with tempering time (at constant temperature) and with increasing temperature (at constant tempering time). The hardness of tempered martensite depends on the ferritecementite phase boundary area; since these phase boundaries are barriers to dislocation motion, the greater the area the harder the alloy. The microstructure of tempered martensite consists of small spherelike particles of cementite embedded within a ferrite matrix. As the size of the cementite particles increases, the phase boundary area diminishes, and the alloy becomes softer. Therefore, with increasing tempering time, the cementite particles grow, the phase boundary area decreases, and the
36 hardness diminishes. As the tempering temperature is increased, the rate of cementite particle growth also increases, and the alloy softens, again, because of the decrease in phase boundary area. Question 10.34: Briefly describe the simplest heat treatment procedure that would be used in converting a 0.76 wt% C steel from one microstructure to the other, as follows: (a) Spheroidite to tempered martensite (b) Tempered martensite to pearlite (c) Bainite to martensite (d) Martensite to pearlite (e) Pearlite to tempered martensite (f) Tempered martensite to pearlite (g) Bainite to tempered martensite (h) Tempered martensite to spheroidite In this problem we are asked to describe the simplest heat treatment that would be required to convert a eutectoid steel from one microstructure to another. Figure is used to solve the several parts of this problem. (a) For spheroidite to tempered martensite, austenitize at a temperature of about 760 C, quench to room temperature at a rate greater than about 140 C/s, then isothermally heat at a temperature between 250 and 650 C. (b) For tempered martensite to pearlite, austenitize at a temperature of about 760 C, then cool to room temperature at a rate less than about 35 C/s. (c) For bainite to martensite, first austenitize at a temperature of about 760 C, then quench to room temperature at a rate greater than about 140 C/s. (d) For martensite to pearlite, first austenitize at a temperature of about 760 C, then cool to room temperature at a rate less than about 35 C/s. (e) For pearlite to tempered martensite, first austenitize at a temperature of about 760 C, then rapidly quench to room temperature at a rate greater than about 140 C/s, then isothermally heat treat (temper) at a temperature between 250 and 650 C. (f) For tempered martensite to pearlite, first austenitize at a temperature of about 760 C, then cool to room temperature at a rate less than about 35 C/s. (g) For bainite to tempered martensite, first austenitize at a temperature of about 760 C, then rapidly quench to room temperature at a rate greater than about 140 C/s, then isothermally heat treat (temper) at a temperature between 250 and 650 C. (h) For tempered martensite to spheroidite simply heat at about 700 C for approximately 20 h.
37 Question 10.35: (a) Briefly describe the microstructural difference between spheroidite and tempered martensite. (b) Explain why tempered martensite is much harder and stronger. (a) Both tempered martensite and spheroidite have spherelike cementite particles within a ferrite matrix; however, these particles are much larger for spheroidite. (b) Tempered martensite is harder and stronger inasmuch as there is much more ferritecementite phase boundary area for the smaller particles; thus, there is greater reinforcement of the ferrite phase, and more phase boundary barriers to dislocation motion.
Composition Solidus Liquidus (wt% Au) Temperature ( C) Temperature ( C)
10.4 Given here are the solidus and liquidus temperatures for the copper gold system. Construct the phase diagram for this system and label each region. Composition Solidus Liquidus (wt% Au) Temperature
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationHW 8. G = a 3 G v. 6a 2. Problem a. To Find:
HW 8 Problem 10. a. To Find: (a) The expression for total free energy change for a cubic nucleus, critical cube edge length, a*, and G* (b) Compare G* for a cube with that for a sphere b. Given: Nucleus
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationChapter 10: Phase Transformations
Chapter 10: Phase Transformations ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC γ (Austenite) Eutectoid transformation Fe 3 C (cementite) + α (ferrite) (BCC) How does the
More informationPhase transformation
Phase transformation Phase Transformation Topics o Basic principles relating to transformations o Kinetics of phase transformation: Nucleation and growth o Metastable and equilibrium state o Shape memory
More informationMATERIALS 101 INTRODUCTION TO STRUCTURE AND PROPERTIES WINTER Problem Set 6 Due: Tuesday, March 6, 11:00 AM
Problem Set 6 Due: Tuesday, March 6, 11:00 AM 1. TTT Diagrams Based on the transformation diagrams for eutectoid steel shown below, what microstructure would result from the following cooling histories?
More information= 62 wt% Ni38 wt% Cu.
92 9.2 (a) From Figure 9.8, the maximum solubility of Pb in Sn at 100 C corresponds to the position of the β (α + β) phase boundary at this temperature, or to about 2 wt% Pb. (b) From this same figure,
More information9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure
913 9.8: 9.11 Upon heating a leadtin alloy of composition 30 wt% Sn70 wt% Pb from 150 C and utilizing Figure (a) The first liquid forms at the temperature at which a vertical line at this composition
More informationProblem Set 7 Materials101 1.) You wish to develop a gold alloy (mostly gold) that can be precipitation strengthened to provide high strength  high conductivity electrical leads to integrated circuits
More informationIntroduction to Materials Science, Chapter 11, Thermal Processing of Metal Alloys. Chapter 11 Thermal Processing of Metal Alloys
Chapter 11 Thermal Processing of Metal Alloys Designer Alloys: Utilize heat treatments to design optimum microstructures and mechanical properties (strength, ductility, hardness.) Strength in steels correlates
More informationLecture 19: Eutectoid Transformation in Steels: a typical case of Cellular
Lecture 19: Eutectoid Transformation in Steels: a typical case of Cellular Precipitation Today s topics Understanding of Cellular transformation (or precipitation): when applied to phase transformation
More informationIntroduction to Iron Metallurgy. Lee Morin Houston Home Metal Shop Club October 2010
Introduction to Iron Metallurgy Lee Morin Houston Home Metal Shop Club October 2010 Book I stole the pictures from We will start with a brief overview! Metals Are Crystals Fundamental geometry of a crystal
More informationIntroduction to Materials Science, Chapter 9, Phase Diagrams. Phase Diagrams. University of Tennessee, Dept. of Materials Science and Engineering 1
Phase Diagrams University of Tennessee, Dept. of Materials Science and Engineering 1 Chapter Outline: Phase Diagrams Microstructure and Phase Transformations in Multicomponent Systems Definitions and basic
More informationThe mechanical properties of metal affected by heat treatment are:
Training Objective After watching this video and reviewing the printed material, the student/trainee will learn the basic concepts of the heat treating processes as they pertain to carbon and alloy steels.
More informationDr. Pulak M. Pandey. paniit.iitd.ac.in/ ~ pmpandey
Dr. Pulak M. Pandey http:// paniit.iitd.ac.in/ ~ pmpandey Metals and alloys may not posses all the desired properties in the finished product. Alloying and heat treatment are two methods which are extensively
More informationModule 34. Heat Treatment of steel IV. Lecture 34. Heat Treatment of steel IV
Module 34 Heat reatment of steel IV Lecture 34 Heat reatment of steel IV 1 Keywords : Austenitization of hypo & hyper eutectoid steel, austenization temperature, effect of heat treatment on structure &
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
14:440:407 Fall 010 Additional problems and SOLUTION OF HOMEWORK 07 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 To provide
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More information3. Apply phase rule to the two phase field of a binary isomorphous diagram. What conclusion can be drawn?
ecture 1822: Solidification of binary alloys: Solidification of binary alloys: limits of solubility, isomorphous system, lever rule, constitutional super cooling, effect of non equilibrium cooling, eutectic,
More informationIntroduction to Structure and Properties Winter 2005 Final Exam March 17, 2005 TOTAL POINTS 37
Materials 101 Introduction to Structure and Properties Winter 005 Final Exam March 17, 005 Solutions TOTAL POINTS 37 Problem 1: Tensile Test and Plastic Deformation (10 Points) A copper rod is deformed
More informationContinuous Cooling Transformation (CCT) Diagrams
Continuous Cooling Transformation (CCT) Diagrams R. Manna Assistant Professor Centre of Advanced Study Department of Metallurgical Engineering Institute of Technology, Banaras Hindu University Varanasi221
More informationHeat Treatment of Steels : Spheroidize annealing. Heat Treatment of Steels : Normalizing
Heat Treatment of Steels :Recrystallization annealing The carbon and alloy steels were treated at a temperature of about 700 C, which is about 20 C below the eutectoid temperature. The holding time should
More informationExperiment: Heat Treatment  Quenching & Tempering
Experiment: Heat Treatment  Quenching & Tempering Objectives 1) To investigate the conventional heat treatment procedures, such as quenching and annealing, used to alter the properties of steels. SAE
More informationLABORATORY EXPERIMENTS TESTING OF MATERIALS
LABORATORY EXPERIMENTS TESTING OF MATERIALS 1. TENSION TEST: INTRODUCTION & THEORY The tension test is the most commonly used method to evaluate the mechanical properties of metals. Its main objective
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationSection 3: HEAT TREATMENT
Section 3: HEAT TREATMENT Introduction Objectives of Heat Treatment Heat Treatment is the controlled heating and cooling of metals to alter their physical and mechanical properties without changing the
More informationModule 4 Design for Assembly IIT BOMBAY
Module 4 Design for Assembly Lecture Design for Heat Treatment 7 Instructional objectives By the end of this lecture, the student will learn 1. different heat treatment processes, 2. application of various
More informationAlloys & Their Phase Diagrams
Alloys & Their Phase Diagrams Objectives of the class Gibbs phase rule Introduction to phase diagram Practice phase diagram Lever rule Important Observation: One question in the midterm Consider the Earth
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationHeat Treatment of Steel
Heat Treatment of Steel Steels can be heat treated to produce a great variety of microstructures and properties. Generally, heat treatment uses phase transformation during heating and cooling to change
More informationPhase Transformations in Metals and Alloys
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationLecture 3: Introduction to Diffusion
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 3: Introduction to Diffusion Mass transport in
More informationChapter 5: Diffusion. 5.1 SteadyState Diffusion
: Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process
More informationLecture 1: Kinetics vs. Thermodynamics: different but related
Lecture 1: Kinetics vs. Thermodynamics: different but related Today s topics The basic concepts of Kinetics and Thermodynamics, and how to understand the difference and interrelationship between the two
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS. C Zn A Cu C Zn A Cu C Cu A Zn. (30)(63.55 g /mol) (30)(63.55 g /mol) (70)(65.
HAPTER 4 IMPERFETIONS IN SOLIDS PROBLEM SOLUTIONS wt% u? 4.7 What is the composition, in atom percent, of an alloy that consists of 30 wt% Zn and 70 4.6 as In order to compute composition, in atom percent,
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationHEAT TREATMENT OF STEEL
HEAT TREATMENT OF STEEL Heat Treatment of Steel Most heat treating operations begin with heating the alloy into the austenitic phase field to dissolve the carbide in the iron. Steel heat treating practice
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 5 Heat Treatment of Plain Carbon and Low
More informationMSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY
MSE 528  PRECIPITATION HARDENING IN 7075 ALUMINUM ALLOY Objective To study the time and temperature variations in the hardness and electrical conductivity of AlZnMgCu high strength alloy on isothermal
More information5 Some standard heat treatments
Part VI. : Heat treatment Module 5 : Some standard heat treatments 5 Some standard heat treatments 5.1 Annealing Consider the TTT diagram as shown in Fig. 9 and the cooling curves imposed on the TTT diagram.
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationMAE 20 Winter 2011 Assignment 6
MAE 0 Winter 011 Assignment 6 8.3 If the specific surface energy for sodalime glass is 0.30 J/m, using data contained in Table 1.5, compute the critical stress required for the propagation of a surface
More informationCHAPTER 11 APPLICATIONS AND PROCESSING OF METAL ALLOYS PROBLEM SOLUTIONS
111 CHAPTER 11 APPLICATIONS AND PROCESSING OF METAL ALLOYS PROBLEM SOLUTIONS Ferrous Alloys 11.1 This question asks that we list four classifications of steels, and, for each, to describe properties and
More informationDevelopment of HighStrength Steel Wire with Superior Weldability
INDUSTRIAL MATERIALS Development of HighStrength Steel Wire with Superior Weldability Hiromu IzumIda*, Kenichi SHImIzu, Shinei TaKamura, Yasuhiro SHImoda, osamu momozawa and Teruyuki murai Highcarbon
More informationBinary phase diagrams
inary phase diagrams inary phase diagrams and ibbs free energy curves inary solutions with unlimited solubility Relative proportion of phases (tie lines and the lever principle) Development of microstructure
More informationChapter 1 Introduction to Material science & Metallurgy
Chapter 1 Introduction to Material science & Metallurgy 1. Material Science & Metallurgy (21419) State the importance of study of materials science and briefly. Explain Engineering requirements of materials.
More informationFundamentals of the Heat Treating of Steel
CHAPTER 2 Fundamentals of the Heat Treating of Steel BEFORE CONSIDERATION can be given to the heat treatment of steel or other ironbase alloys, it is helpful to explain what steel is. The common dictionary
More informationLecture 18 Strain Hardening And Recrystallization
138 Lecture 18 Strain Hardening And Recrystallization Strain Hardening We have previously seen that the flow stress (the stress necessary to produce a certain plastic strain rate) increases with increasing
More informationProblem Set 4 Solutions
Chemistry 360 Dr Jean M Standard Problem Set 4 Solutions 1 Two moles of an ideal gas are compressed isothermally and reversibly at 98 K from 1 atm to 00 atm Calculate q, w, ΔU, and ΔH For an isothermal
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationTHE STRUCTURE OF CRYSTALLINE SOLIDS
CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS PROBLEM SOLUTIONS Fundamental Concepts 3.1 What is the difference between atomic structure and crystal structure? Atomic structure relates to the number of
More informationConcepts of Stress and Strain
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original
More informationSample Exercise 14.1 Calculating an Average Rate of Reaction
Sample Exercise 14.1 Calculating an Average Rate of Reaction From the data given in the caption of Figure 14.3, calculate the average rate at which A disappears over the time interval from 20 s to 40 s.
More informationChapter Biography of J. C. Maxwell Derivation of the Maxwell Speed Distribution Function
Chapter 10 10.1 Biography of J. C. Maxwell 10.2 Derivation of the Maxwell Speed Distribution Function The distribution of molecular speeds was first worked out by Maxwell before the development of statistical
More informationCHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS
CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a freebody diagram),
More information14:635:407:02 Homework III Solutions
14:635:407:02 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 327 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationAP Physics Problems Kinetic Theory, Heat, and Thermodynamics
AP Physics Problems Kinetic Theory, Heat, and Thermodynamics 1. 19746 (KT & TD) Onetenth of a mole of an ideal monatomic gas undergoes a process described by the straightline path AB shown in the pv
More informationUNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121. Spring Semester 2008 Professor R.
UNIVERSITY OF CALIFORNIA College of Engineering Department of Materials Science & Engineering MSE 121 Spring Semester 2008 Professor R. Gronsky Exam Instructions Please PRINT your name in the box above
More informationINFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES
COMATTECH 2005 TRNAVA, 2021 October 2005 INFLUENCE OF THERMOMECHANICAL TREATMENT ON THE STEEL C45 FATIGUE PROPERTIES Jiří MALINA 1+2, Hana STANKOVÁ 1+2, Jaroslav DRNEK 3, Zbyšek NOVÝ 3, Bohuslav MAŠEK
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationPhase Equilibria & Phase Diagrams
Phase Equilibria & Phase Diagrams Week7 Material Sciences and Engineering MatE271 1 Motivation Phase diagram (Ch 9) Temperature Time Kinematics (Ch 10) New structure, concentration (mixing level) (at what
More informationIntroduction To Materials Science FOR ENGINEERS, Ch. 5. Diffusion. MSE 201 Callister Chapter 5
Diffusion MSE 21 Callister Chapter 5 1 Goals: Diffusion  how do atoms move through solids? Fundamental concepts and language Diffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities Diffusion
More informationEffect of Heat Treatment Processes on the Mechanical Properties of Medium Carbon Steel
Journal of Minerals & Materials Characterization & Engineering, Vol. 11, No.2 pp.143152, 2012 jmmce.org Printed in the USA. All rights reserved Effect of Heat Treatment Processes on the Mechanical Properties
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationComparison of Three NiHard I Alloys
Comparison of Three NiHard I Alloys Ö. N. Do an 1, J.A. Hawk 1, and J.Rice 2 1 U.S. Department of Energy, Albany Research Center, Albany, Oregon 2 Texaloy Foundry Co., Inc., Floresville, Texas Keywords:
More informationFor the M state, n = 3, and 18 states are possible. Possible l values are 0, 1, and 2; possible m l. values are 0, ±1, and ±2; and possible m s
.6 Allowed values for the quantum numbers of electrons are as follows: n 1,,,... l 0, 1,,,..., n 1 m l 0, ±1, ±, ±,..., ±l m s ± 1 The relationships between n and the shell designations are noted in Table.1.
More informationStructure of Metals 110
Structure of Metals 110 Welcome to the Tooling University. This course is designed to be used in conjunction with the online version of this class. The online version can be found at http://www.toolingu.com.
More informationTHE WAY TO SOMEWHERE. Subtopics. Diffusion Diffusion processes in industry
THE WAY TO SOMEWHERE Subtopics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
More informationPhase. Gibbs Phase rule
Phase diagrams Phase A phase can be defined as a physically distinct and chemically homogeneous portion of a system that has a particular chemical composition and structure. Water in liquid or vapor state
More informationIn the metals industry, there are numerous steps
How annealing, stress relief and aging each affect the mechanical properties of spring materials By Terry Bartel Elgiloy Specialty Metals In the metals industry, there are numerous steps from the raw material
More informationBINARY SYSTEMS. Definition of Composition: Atomic (molar) fraction. Atomic percent. Mass fraction. Mass percent (weight percent)
BINARY SYSTEMS Definition of Composition: Atomic (molar) fraction Atomic percent Mass fraction Mass percent (weight percent) na =, x i n = A i i i Weight percent mainly in industry! x at % A = x 100 A
More informationLecture: 33. Solidification of Weld Metal
Lecture: 33 Solidification of Weld Metal This chapter presents common solidification mechanisms observed in weld metal and different modes of solidification. Influence of welding speed and heat input on
More information(10 4 mm 2 )(1000 mm 3 ) = 10 7 mm = 10 4 m = 6.2 mi
CHAPTER 8 DEFORMATION AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 8.1 To provide some perspective on the dimensions of atomic defects,
More informationExperiment: Crystal Structure Analysis in Engineering Materials
Experiment: Crystal Structure Analysis in Engineering Materials Objective The purpose of this experiment is to introduce students to the use of Xray diffraction techniques for investigating various types
More informationMaterial Strengthening Mechanisms. Academic Resource Center
Material Strengthening Mechanisms Academic Resource Center Agenda Definition of strengthening Strengthening mechanisms Grain size reduction Solid solution alloying Cold Working (strain hardening) Three
More informationCONCEPT CHECK QUESTIONS AND ANSWERS. Chapter 2 Atomic Structure and Interatomic Bonding
CONCEPT CHECK QUESTIONS AND ANSWERS Chapter 2 Atomic Structure and Interatomic Bonding Concept Check 2.1 Question: Why are the atomic weights of the elements generally not integers? Cite two reasons. Answer:
More information8. Technical Heat Treatment
8. Technical Heat Treatment 8. Technical Heat Treatment 95 6 cm 4 2 02 4 C 400 C C 614 1210 86 42 0 2 cm 6 723 C temperature C 1750 750 250 When welding a workpiece, not only the weld itself,
More informationThis is the 11th lecture of this course and the last lecture on the topic of Equilibrium Carrier Concentration.
Solid State Devices Dr. S. Karmalkar Department of Electronics and Communication Engineering Indian Institute of Technology, Madras Lecture  11 Equilibrium Carrier Concentration (Contd.) This is the 11th
More information[ A] 2. [ A] 2 = 2k dt. [ A] o
Chemistry 360 Dr Jean M Standard Problem Set 3 Solutions The reaction 2A " P follows secondorder kinetics The rate constant for the reaction is k350 0 4 Lmol s Determine the time required for the concentration
More informationTHREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL. Hossam Halfa
THREE MAIN SOLIDIFICATION REACTIONS OF VANADIUM MODIFIED T1 TUNGSTEN HIGH SPEED TOOL STEEL Hossam Halfa Steel Technology Department, Central Metallurgical R&D Institute (CMRDI), Helwan, Egypt, hossamhalfa@cmrdi.sci.eg;
More informationKinetics of Phase Transformations: Nucleation & Growth
Kinetics of Phase Transformations: Nucleation & Growth Radhika Barua Department of Chemical Engineering Northeastern University Boston, MA USA Thermodynamics of Phase Transformation Northeastern University
More informationDamasteel s martensitic stainless Nitrobe 77 is a powder based steel which solves two classical knife problems:
Damasteel s martensitic stainless Nitrobe 77 is a powder based steel which solves two classical knife problems: Sharp edges on chef knives. Nitrobe 77 is dishwasher safe without risk of corrosion or edge
More informationAustempering Heat Treatment of AISI 4340 Steel and Comparative Analysis of Various Physical Properties at Different Parameters
Austempering Heat Treatment of AISI 4340 Steel and Comparative Analysis of Various Physical Properties at Different Parameters Najeeb Niazi 1,*, Salman Nisar 1 and Aqueel Shah 1 1 Department of Manufacturing
More information1. Introduction to thermodynamics a. What is thermodynamics?
1. Introduction to thermodynamics a. What is thermodynamics? Thermodynamics is a description of material properties as a function of state. What do we mean by state? A macroscopic state of a homogeneous
More information( 1+ I K I. λ = v P σ 2. z 11. = N 1 V σ 2 v Z 11. = 1 2 ( N 1 V ) 2 σ 2 v. J = D ( x ) D = 1 3 λ v D = r 2. 2(dimension)t. where K m,app.
Physical Chemistry I Final Exam Name: KEY CHEM 4641 Fall 2013 median = average = 18 /30 high = 30 /30 7 problems worth a total of 30 points. Show your work. Gas constant: R = 8.314 J mol 1 K 1 = 0.08314
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationCHEM N6 November 2014
CHEM1002 2014N6 November 2014 Consider the pressure/temperature phase diagram of H 2 O shown below. 6 Pressure / atm (not to scale) 1 solid A liquid B C gas 0 100 Temperature / C (not to scale) Which
More informationHIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT
IJMC142442 HIGH STRENGTH DUCTILE IRON PRODUCED BY THE ENGINEERED COOLING: PROCESS CONCEPT Copyright 215 American Foundry Society Abstract Simon N. Lekakh Missouri University of Science and Technology,
More informationMAE 20 Winter 2011 Assignment 2 solutions
MAE 0 Winter 0 Assignment solutions. List the point coordinates of the titanium, barium, and oxygen ions for a unit cell of the perovskite crystal structure (Figure.6). In Figure.6, the barium ions are
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationEffect of Heat Treatment on the Microstructure and Mechanical Properties of Steel
金属材料及热处理 学生实验报告范例课程编号 :030107 课程主讲及实验课指导教师 : 刘国权黄鹏 Effect of Heat Treatment on the Microstructure and Mechanical Properties of Steel Song Zhen 40531165 University of Science and Technology Beijing, Dept.of
More informationSteel and cast iron. Chapter Chapter 112
Steel and cast iron Chapter 111 Chapter 112 1 Taxonomy of Metals Metal Alloys Ferrous Steels Cast Irons
More informationUniversity of Cambridge, Materials Science & Metallurgy. Dilatometry
University of Cambridge, Materials Science & Metallurgy H. K. D. H. Bhadeshia Dilatometry The dilatometric method utilises either transformation strains or thermal strains; the basic data generated are
More informationWELDING AND COATING METALLURGY
WELDING AND COATING METALLURGY 1 INTRODUCTION 4 1.1 ROLE OF CARBON IN STEEL 4 1.2 WELDABILITY OF STEELS 5 2 CRYSTAL STRUCTURE 7 2.1 SOLUBILITY OF CARBON 8 3 IRON  IRON CARBIDE PHASE DIAGRAM 9 3.1 AUSTENITE
More informationComparison of Impact Properties for Carbon and Low Alloy Steels
J. Mater. Sci. Technol., 2011, 27(10), 931936. Comparison of Impact Properties for Carbon and Low Alloy Steels O.H. Ibrahim Metallurgy Dept., Nuclear Research Centre, Atomic Energy Authority, Egypt [Manuscript
More information